Download presentation

Presentation is loading. Please wait.

Published byTate Bugg Modified over 2 years ago

1
The physics of blue lasers, solar cells, and stop lights Paul Kent University of Cincinnati & ORNL

2
The physics of blue lasers, solar cells, and stop lights Paul Kent Solid State Theory Group National Renewable Energy Laboratory U.S. Department of Energy Office of Science Basic Energy Sciences Division of Materials Sciences Thanks to: Alex Zunger & SST Group/Basic Sciences

3
Outline 1. Introduction Nitride semiconductors Novel phenomena. Localized states 2. How can we model these systems? Computational techniques 3. New photovoltaic materials GaAsN (and GaPN) Band gap reduction. Localized states 4. Blue emitters InGaN Localization at In inhomogeneities

4
Blue laser Sony 30GB DVD High brightness LEDs Traffic signals. Solid state lighting? High efficiency photovoltaics? InGaN InGaN, AlGaN… GaAsN GaAs/Ge 19% eff.

5
Absorption in semiconductors Conduction band Valance band (occupied states) Energy Photon h

6
High Efficiency Multijunction Solar Cells Want 1 eV material lattice- matched to GaAs Try GaInNAs Calculated efficiencies (ideal) 500X AM1.5D:36%47%52% one sun AM0:31%38%41%

7
Isostructural semiconductor alloying Properties approx. a linear combination of the components

8
Anomaly #1: Band gap reduction in GaAsN Band gap reduced by ~120meV per % nitrogen! Shan et al. Phys. Rev. Lett. 82 1221 (1999) No nitrogen 0.9 % 2 % Band gaps GaAs ~1.5 eV GaN ~3.5 eV 1.2 %

9
Anomaly #2: Dilute Nitrogen in GaAs Many sharp lines seen in emission! Liu, Pistol and Samuelson. Appl. Phys. Lett. 56 1451 (1990) T. Makimoto et al. Appl. Phys. Lett. 70 2984 (1997) GaAs:N Wavelength (nm) NN 1 0 kbar 1 kbar

10
Outline 1. Introduction Nitride semiconductors Novel phenomena. Localized states 2. How can we model these systems? Computational techniques 3. New photovoltaic materials GaAsN (and GaPN) Band gap reduction. Localized states 4. Blue emitters InGaN Localization at In inhomogeneities

11
Simplified view of a semiconductor alloy Simulate regular lattices Distributions of atoms 10^3-10^6 atoms required Atomic relaxation important

12
Computational Modeling of Alloys Use large supercells (10^3-10^6 atoms) containing many nitrogens Statistically average properties of many random configurations Use Valence Force Field for structural relaxation Use Empirical Pseudopotential Method for wavefunctions Small Supercell Approach Large Supercell Approach

13
Folded Spectrum Method (FSM) valence states conduction states 1 4 2 3 5 N-4 N-1 N-3 N-2 N 1 4 2 3 5 1 4 2 3 5 “Fold” States ref Band Gap valence states conduction states Only calculate “interesting” states around band gap Wang & Zunger J. Chem. Phys. (1994) Recently: Jacobi-Javidson Tackett PRB (2002) 1

14
Outline 1. Introduction Nitride semiconductors Novel phenomena. Localized states 2. How can we model these systems? Computational techniques 3. New photovoltaic materials GaAsN (and GaPN) Band gap reduction. Localized states 4. Blue emitters InGaN Localization at In inhomogeneities

15
High Efficiency Multijunction Solar Cells Want 1 eV material lattice- matched to GaAs Try GaInNAs Calculated efficiencies (ideal) 500X AM1.5D:36%47%52% one sun AM0:31%38%41%

16
Anomaly #1: Band gap reduction in GaAsN Band gap reduced by ~120meV per % nitrogen! Shan et al. Phys. Rev. Lett. 82 1221 (1999) No nitrogen 0.9 % 2 % Band gaps GaAs ~1.5 eV GaN ~3.5 eV 1.2 %

17
Anomaly #2: Dilute Nitrogen in GaAs Many sharp lines seen in emission! Liu, Pistol and Samuelson. Appl. Phys. Lett. 56 1451 (1990) T. Makimoto et al. Appl. Phys. Lett. 70 2984 (1997) GaAs:N Wavelength (nm) NN 1 0 kbar 1 kbar

18
N in GaAs, GaP 1. Isolated Nitrogen 2. Pairs and clusters 3. Well-developed alloys I will discuss three cases:

19
GaP:N Nitrogen localized a 1 (N) In GaP:N (0.01%): Level ~30 meV below CBM Introduces character Any concentration of nitrogen in GaP creates “direct gap” character

20
A1 Levels of Isolated Impurity GaAs:N 44 Angstrom 4096 atoms / L / X (%) Nitrogen localized level ~ 150 meV inside conduction band Localized Level in GaAs:N

21
N in GaAs, GaP 1. Isolated Nitrogen 2. Pairs and clusters 3. Well-developed alloys

22
N Clusters in GaAs, GaP 1. Ga(P m N 4-m ) Clusters 2. [1,1,0]-Oriented Nitrogen Chains 1 N 2 N 3 N4 N [1,1,0] NNN N N

23
Energy levels of Clusters and Chains in GaP

24
N in GaAs, GaP 1. Isolated Nitrogen 2. Pairs and clusters 3. Well-developed alloys

25
E CBE = Delocalized Conduction Band Edge

27
GaPN

28
GaAsN

29
Two types of state observed Dilute Limit:PHS in conduction band and pair/cluster CS in gap Intermediate Range:CS do not move PHS plunge down in energy Amalgamation Point:Lowest energy PHS just below CS

30
Anticrossing/repulsion between band edge and localized states drives band gap down Band gap reduction

31
GaPN Pressure dependence –14 meV/GPa Pressure Energy Bulk GaP

32
Red Shift of PL vs PLE Majority state absorbs Minority state emits I. A. Buyanova et al. MRS IJNSR 6 2 (2001) - Emission from localized minority states - Absorption to majority states

33
Summary: GaAsN & GaPN 2. Cluster states are fixed in energy 3. Host states move down, overtaking the cluster levels, one-by-one Host states repelled from nitrogen resonant levels 4. Both localized and delocalized states exist at the band edge 1. Small nitrogen aggregates create near-gap levels Some “cluster state” levels are deep, even for small aggregates Kent & Zunger Phys. Rev. Lett. 86 2613 (2001) Kent & Zunger Phys. Rev. B 64 5208 (2001) Kent & Zunger Appl. Phys. Lett. 79 2339( 2001)

34
Outline 1. Introduction Nitride semiconductors Novel phenomena. Localized states 2. How can we model these systems? Computational techniques 3. New photovoltaic materials GaAsN (and GaPN) Band gap reduction. Localized states 4. Blue emitters InGaN Localization at In inhomogeneities

35
Zinc-Blende InGaN Alloys Despite large defect density InGaN alloys emit Time resolved PL – many length (time) scales Theory: Bulk InGaN alloys emit weakly Q. What is the role of In inhomogeneity? Why is emission so efficient?

36
InGaN band offsets

37
Experimental Observations 15% In 20% In 25% In HRTEM InGaN MQW Lin et al. APL 77 2988 (2000) Lemos et al. PRL 84 3666 (2000) ~300 meV+ lowering in emission energy in 33% c-InGaN samples 10nm

38
InGaN Intrinsic Dot Calculations Spherical dot in 141000 atom supercell Dot: High In composition 80%+ Alloy supercell: Lower In composition 33% Electrons Quantum confined on dot Holes Localized in/near dot (strain, alloy fluctuations)

39
Calculations of Intrinsic Dots Small In-rich regions give large “band gap” reduction

40
Hole Localization in Random Alloys Holes localize near (statistically occurring) (1,1,0)-oriented Indium chains! 1000 atom supercell 20% In

41
Indium fluctuations are key Localized states occur near VBM, CBM } “Quantum dot” states due to inhomogeneity

42
Summary: InGaN Indium fluctuations are key - localization easily results => Can specify quality of growth required for opto devices Kent & Zunger Appl. Phys. Lett. 79 1977 (2001) Small (~30 A) In-rich (80%+) regions cause low energy PL Localized hole states exist even in random alloy

43
Conclusion prc.kent@physics.org 1. Nitride alloys display “new physics” due to formation of localized states 2. Large-scale computational modeling can help explain nitride properties http://www.physics.uc.edu/~pkent

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google